Applications of bulk ferroelectrics
Consider an insulating system with non-zero spontaneous polarization
The enormously broad range of materials exhibiting ferroelectricity and the variety of their physical properties result in numerous applications of bulk ferroelectrics . Table 1 shows the connections between different physical effects exhibited by bulk ferroelectrics and their applications.
Recent advances in nanotechnologies, especially in nanoinstrumentation (for example, scanning probe microscopy ) and materials nanofabrication , allowed the direct probing of ferroelectricity at the nanoscale. The new and unexplored world of nanoscale ferroelectrics (nanoparticles of different shapes and sizes, nanofilms, nanopatterned structures, etc.) raised fundamental questions and stimulated very active research in both academic and industrial sectors . As a result, a new era of nanoscale ferroelectrics was launched. Novel effects, associated with reduced dimensions and found in nanoscaleferroelectrics, highlighted exciting possibilities for new applications reviewed recently in . Almost all of the attention for the mentioned review  was devoted to the
|Ferroelectric hysteresis||Nonvolatile computer information storage|
|High relative permittivities (several thousands)||Capacitors|
|Direct piezoelectric effect||Sensors (microphones, accelerometers, hydrophones, etc.)|
|Converse piezoelectric effect||Actuators, ultrasonic generators, resonators, filters|
|Pyroelectric effect||Uncooled infra-red detectors|
|Electro-optic effects||Laser Q-switches, optical shutters and integrated optical (photonic) devices|
|Nonlinear optical effects||Laser frequency doubling, optical mixing, including four-wave mixing and holographic information storage|
|Coupling between stress and birefringence||Radar signal processing|
|Positive temperature coefficient of resistance (PTCR)||Electric-motor overload-protection devices and self-stabilizing ceramic heating elements|
2. Methods of ferroelectric nanoparticles production: Nano-powders and nano-colloids
The existing methods that produce ferroelectric nanoparticles are numerous and can be classified as physical, chemical, and biological (Fig. 1). The primary goal of each method is to control size, shape, morphology, and crystallinity of nanoparticles to produce a desirable effect. This task represents a real challenge, and, as a result, there are no well-defined boundaries between physical, chemical, or biological methods. Moreover, in many cases, a combination of at least two methods (for example, physical and chemical methods, i.e. a physical-chemical approach) is required in order to fabricate good quality particles (small sizes, narrow size distribution, ferroelectric phase).
2.1. Chemical methods
The most widely used chemical methods for the synthesis of ferroelectric nanoparticles are: 1) solid-state reaction; 2) sol-gel technique; 3) solvothermal method; 4) hydrothermal method; and 5) molten salt method.
Table 2 shows selected examples of these methods applied to synthesis of ferroelectric nanoparticles of BaTiO3. As can be seen from Table 2, the ultra-fine ferroelectric nanoparticles (<10 nm) in almost all cases except  are synthesized in a cubic phase which is not ferroelectric. The tetragonal phase (with ferroelectric response) is possible for relatively large particles (~50-70 nm). This fact can be critical for certain types of applications, and will be discussed later.
|Wet chemical route at low temperature (50°C);
H2TiO3 nanotubes; ethanol/water mixture with 25% ethanol by volume; Ba(OH)2·8H2O
|Uniform BaTiO3 nanotubes, a
Powder X-ray diffraction (XRD), field-emission scanning electron microscopy (FE-SEM),
transmission electron microscopy (TEM), Raman spectroscopy, and X-ray photoelectron spectroscopy
|Promising microwave-absorbing materials|
Barium titanium ethyl hexano-isopropoxide, BaTi(O2CC7H15)(OCH(CH3)2)5 ; a mixture of diphenyl ether, (C5H5)2O; stabilizing agent oleic acid, CH3(CH2)7CHdCH(CH2)7-
CO2H, at 140 °C, under argon or nitrogen
nanoparticles with diameters ranging from 6 to 12 nm,
|Multilayer ceramic capacitors|
|Dense polycrystalline aggregates (~80 nm) of nanocrystals
|Solid-state reaction as a function of temperature (400–8000C), time (1–24 hr);
Nanocrystalline TiO2, ultrafine BaCO3 and submicrometer BaCO3 were intensively mixed in an aqueous suspension for 24 hr using polyethylene jars and zirconia media. The polymer (ammonium polyacrylate) was required for the formation of a monolayer on the particle surface
|Nanoparticle size is 70 nm. Specific surface area up to ~15m2/g,
TG and DTA analysis, XRD, SEM
|Multilayer ceramic capacitors|
|Polyhedral with hexagonal outline in shape;
|Molten salt method;
Hydroxide octahydrate (Ba(OH)2·8H2O), titanium dioxide (TiO2), and the eutectic salts (NaCl–KCl), 600-900 °C
XRD, Fourier transform infrared spectrometry, UV–Vis diffuse reflectance spectra, and field emission SEM
|Nanoparticles are well dispersed|
|Single crystalline nanoparticles;
Ba(CH3COO)2 and Ti(OC4H9)4 ; the autoclave was maintained at
200 °C for 12 hr
XRD, TEM, SAED, FTIR
|Dense bulk nanocomposites|
(Ba,Sr)(OiPr)2, Ti(OiPr), EtOH,
330–400 °C, 16-30 MPa
|Dense bulk nanocomposites|
|Combined wet-chemical and rapid calcination process;
Ec = 4.91 kV/cm; (cigar-like loop);surface area 7.96 m2/g
XRD, TEM, TGA, SMPS, SAED,dielectric spectroscopy
|Multilayer ceramic capacitor|
|One-step solvothermal route;
Tetra-n-butyl titanate, Barium hydroxide octahydrate, solvent (Diethylene glycol), surfactant (Polyvinyl Pyrrolidone)
XRD, TEM, HRTEM, Raman spectroscopy
|Multilayer ceramic capacitor|
2.2. Physical methods
Dry and wet mechanical grindings are methods of choice for inexpensive nanoparticle preparation. For technological applications, wet grinding is preferable because it allows more options to control the size of the nanoparticles. During the last few years, substantial progress was made in the field of ferroelectric nanoparticle preparation by means of wet mechanical grinding . Generally, three components are needed: raw material to grind (micron-sized powders of BaTiO3); surfactant (which covers the particle surface and prevents their aggregation and overheating during grinding; oleic acid is a good choice for BaTiO3); and fluid carrier (both raw material and surfactant are mixed with fluid carrier; heptane is widely used to grind BaTiO3). An extensive list of references, as well as recent achievements in the field, are discussed in the review . Table 3 shows how particle sizes depend upon grinding time .
As is seen from Table 3, wet mechanical grinding can produce 9 nm nanoparticles, and such small particles are still in ferroelectric phase. It is important to remember that BaTiO3 nanoparticles of the same sizes synthesized by the majority of chemical methods are not ferroelectric – the method used to fabricate nanoparticles really does matter. The ability to produce ferroelectric nanoparticles of very small sizes is a defining characteristic of this physical method (see  for more references).
The net dipole moment of ferroelectric nanoparticles allows them to be harvested by using an inhomogeneous electric field. The harvesting concept proposed in  is based on the fact that dipoles experience a translational force only when exposed to a field gradient. For a given linear field gradient and assuming a single ferroelectric domain, the net translational force on a dipole scales proportionally with the particle size. The Brownian motion effects also become progressively more pronounced at smaller particle sizes and so the required field strength for successful separation scales nonlinearly as the particle size is reduced.
Both gas-phase and liquid-phase harvesting methods were proposed and tested successfully, and single ferroelectric monodomain nanoparticles as small as 9 nm from mechanically ground nanoparticles were selectively harvested . In contrast to many reports on the lack of ferroelectricity for nanoparticles below 10 nm (see Table 2), the harvested nanoparticles do maintain ferroelectricity. The ferroelectric response of such tiny nanoparticles was attributed to the existence of an induced surface strain as a result of the grinding process . The lack of a mechanically induced strain in similarly sized but chemically produced nanoparticles accounts for the absence of ferroelectricity in these materials. The concept of stress-induced ferroelectricity was verified in further experiments, which are reviewed in . It was found  that the spontaneous polarization of the nanoparticles is four to five times larger than the spontaneous polarization of the bulk raw materials. To obtain this result the following two conditions must be satisfied: (1) a nonpolar solvent for the nanoparticle suspension and (2) nonaggregated nanoparticles. Under these conditions, for 9 nm nanoparticles, the values of 100–120 µC/cm2 and 8.9 10-23C cm have been measured for the spontaneous polarization and dipole moment, respectively. The aggregation of ferroelectric nanoparticles masks the ferroelectric response due to the partial compensation of the dipole moments of the individual particles. Finally, we can conclude that recent advances in the production of uniform, monodomain, highly ferroelectric nanoparticles indicate that this field has reached its maturity. The particles can now be reliably prepared to certain specifications and characteristics .
2.3. Physical-chemical methods
In order to prepare ferroelectric nanoparticles with controllable sizes and shapes a combination of chemical methods with external physical factors (for example, a chemical reaction in the presence of electromagnetic fields or mechanical milling) is needed. Table 4 shows several examples of these physical-chemical methods for the case of BaTiO3.
As can be seen from Table 4, chemical reactions under the presence of an external driver (microwave, ultrasonic, milling, heat, pressure) are able to produce very fine particles (~5-10 nm) with tetragonal structures.
|Microwave (2.45 GHz, output power ~ 800W) hydrothermal;
barium nitrate (Sigma Aldrich, purity ≥99.99%), titanium isoproxide
(Sigma Aldrich, purity ≥97%), nitric acid (ACS reagent 70%), ammonium hydroxide (Sigma Aldrich), and glycine (Sigma-Aldrich, purity ≥99%)
|Cross section 70 ± 9 nm in  projection;
XRD, high resolution TEM, impedance spectroscopy
|Charge storage devices|
|Nearly spherical nanoparticles;
|Sol–gel-hydrothermal method under an oxygen (partial pressure is ~60 bar);
TiCl4; HCl; BaCl2·2H2O; deionized water, stirring and N2 bubbling, NaOH
|Sizes range from 50 to 75nm; transition
of BaTiO3 from
Ec = 3.2 kV/cm (cigar-like loop);
XRD, TEM, Raman and dielectric spectroscopy; energy-dispersive X-ray spectroscopy; AFM
|Oxygen atmosphere decreases sizes of the nanoparticles (for example , at 200 °C sizes decrease from 72.54 nm to
|Direct synthesis from solution
(DSS) – mechanochemical synthesis;
Anhydrous Ba(OH)2 and tetrabutyl titanate [Ti (OC4H9)4]
Mechanical milling at the rate of 200 rpm, room temperature
XRD, TEM, Raman spectroscopy
|Chemical reaction during milling|
|Large aggregates of 5–10 nm small nanocrystals;
BaCl2 ; TiCl4; NaOH
|100 nm aggregates,
XRD, TEM, DLS, SAED
|Multilayer ceramic capacitors|
|RF-Plasma chemical vapor deposition (CVD);
iso-propoxide (Ti(OiPr)4, bis-dipivaloylmethanate (Ba(DPM)2
XRD, TEM, SAED, EDX
|Multilayer ceramic capacitors|
[28, 29, 30]
barium acetate, PVP, titanium isopropoxide, ethanol, acetic acid
|80-190 nm in diameter, 0.1 mm in length;
XRD, TEM, SAED
|Piezo, microwave material, sensors, capacitors|
|Flame spray pyrolysis;
barium carbonate and titanium tetra-
XRD, TEM, SEM
|Multilayer ceramic capacitors|
Another interesting subject is the possible application of ceramic nanofibers produced by the method of electrospinning. These possible applications include: nanofiber-based supports for catalysts, nanofiber-based photocatalysts, nanofiber-based membrane for filtration, nanofiber-based sensors, nanofiber-based photoelectrodes for photovoltaic cells, nanofiber-based electrodes for lithium batteries, nanofiber-based electrode-supports for fuel cells, and materials for implants [28, 29, 30].
2.4. Biological methods
The proper combination of chemical and physical methods (Table 4) allows the production of very small ferroelectric nanoparticles (5-10 nm). However, toxic chemicals and/or high temperatures/pressures are needed in most cases. These requirements substantially limit the possible biomedical applications of ferroelectric nanoparticles. Biological methods were proposed as eco-friendly “green” alternatives to existing chemical and physical methods. The biosynthesis of different types of nanoparticles was reviewed recently in a few papers [32, 33, 34, 35], but biological methods that produce specifically ferroelectric nanomaterials are not very numerous. For example, the first review  lists nearly a hundred variations for the synthesis of nanoparticles by microorganisms, and only a few of them produce ferroelectric nanoparticles. The biological methods applied to synthesize the nanoparticles of the most widely known ferroelectric BaTiO3 are summarized in Table 5 (papers published before 2008 were discussed in ). The references listed in this table show that most of the biological methods mentioned employ some chemical or physical steps as well.
|Aggregates (~500 nm) of nanocrystals(~ 50 nm);
|The peptides BT1 and BT2induce the room-temperature
Aqueous precursor solution composed of barium acetate (Ba(OOCCH3)2) potassium bis(oxalato) oxotitanate(IV) (K2[TiO(C2O4)2]2H2O); pH 6.8
Pr ~ 2-3 C/cm2; the coercive field,
Ec = 5-6 kV/cm (cigar-like loop);
SEM, TEM, SAED and XRD analysis, dielectric measurements
|Rapid room-temperature synthesis of ferroelectric (tetragonal) BaTiO3 within 2 hr|
BaCO3 and TiO2 solid state synthesis BaTiO3; Slush of micron-sized BaTiO3 particles+ Lactic acid Bacillus
(CH3COO)2Ba and K2TiF6 + fungal micelles of
XRD, DCS, TEM, SAED, XPS, SPM
|Peptide nanorings used as templates;
AFM, TEM, XRD, EFM, Raman
biosynthesis of BaTiO3 nanoparticles;
BaCO3 and TiO2 solid state synthesis BaTiO3, Slurry of large BaTiO3 + yeast culture
|8-21 nm, s
|Kinetically controlled vapor diffusion
Single source, bimetallic alkoxide with the vapor diffusion of a hydrolytic catalyst (H2O)
One can note from Table 5 that these biological methods can be roughly grouped into two categories: the synthesis of ferroelectric nanoparticles using a number of seed chemicals and some type of biological or bio-inspired system, and the creation of nanoparticles using large particles of ready ferroelectric material and some type of biological system. Most of the methods that are currently available fall into the first category; the methods in the second category have appeared only very recently.
The earliest discoveries of nanoparticle synthesis by microorganisms (fungus,
Peptide nanorings provide another interesting biomimetic route to the template-mediated synthesis of BaTiO3 and SrTiO3 nanoparticles . Developed in 2006, it was the very first method of obtaining ferroelectric barium titanate nanoparticles at room temperature (many previous room-temperature methods had trouble growing barium titanate not in the cubic phase).
In this category of biological methods, one has to mention bioinspired methods of dispersing nanoparticles and producing stable colloids. Take for examplethe production of stable nanoparticle suspensions using microbial-derived surfactants  where usual garden variety surfactants are replaced with bio-derived materials that are significantly smaller in size and that help prevent aggregation of multiple nanoparticles during sol-gel synthesis. This process relies on some physical/chemical steps, just like the majority of other biological methods of ferroelectric nanoparticle production that have been developed to date.
These bio-inspired methods show great promise because they produce relatively small ferroelectric nanoparticles at room (or low) temperature compared to conventional physical and chemical methods, many of which require lengthy processes, use of high temperatures, harsh chemicals, etc.
3. Applications of ferroelectric nanoparticles in materials technologies
3.1. Multilayered capacitors and nanocomposites
As was previously mentioned in the introduction, the era of applied ferroelectricity was launched after the first reliable ferroelectric material – ceramic BaTiO3 – was discovered . The very high dielectric constants (~1000) of bulk ferroelectric materials were applied in the manufacturing of discrete and multilayered ceramic capacitors. Advances in the production of ferroelectric nanoparticles broadened this application to a large extent. Currently, nanosized BaTiO3 powders are successfully used for manufacturing miniaturized and highly volume-efficient multilayer ceramic capacitors (MLCCs, for more details see review ).
Typical MLCCs utilize pellets of nanopowders sintered at high temperatures, producing structures with high rigidity that can impose certain limitations. Nanocomposites made of flexible polymers and ferroelectric nanoparticles overcome the restrictions caused by rigidity of sintered structures. Polymeric materials doped with ferroelectric nanoparticles are of considerable interest as a solution for processable high permittivity materials for various electronic applications: volume efficient multilayer capacitors, high-energy-density capacitors, embedded capacitors, and gate insulators in organic field effect transistors .
Both components (polymer and ferroelectric nanoparticle) of such nanocomposites are essential. The polymeric material brings flexibility and the ability to cover a large surface area, while nanoparticles share high values of dielectric permittivity with the matrix-enhancing effective dielectric permittivity of the composite. It’s not easy to achieve homogeneous dispersion of ferroelectric nanoparticles in a polymeric matrix because of the high surface energy of nanoparticles, which usually leads to aggregation and phase separation, resulting in poor processability of the films and a high defect density. In order to make high-quality nanocomposites (good solution processability, low leakage current, high permittivity, and high dielectric strength), surface modification of nanoparticles is needed. The surface modification of nanoparticles decreases attractive forces between them, thus preventing aggregation. In addition, the proper design of a surface agent can increase interactions between the nanoparticles and the polymeric matrix. As a result, a quite homogeneous distribution of the nanoparticles in the polymeric matrix can be achieved. However, there are several obstacles that prevent nanocomposites “polymer/ferroelectric nanoparticle” from mass commercialization. The most common are poor temperature stability of dielectric constants and large dielectric losses. The proper design of both the nanoparticles (material size, shape, surface modification) and the polymer matrix can overcome these problems. For example, Table 6 shows short descriptions of the relatively successful (in terms of material performance) nanocomposites “polymer/BaTiO3”. All of them are optically transparent, have high dielectric permittivity (25-30), and moderate losses (loss tangent is in the range 0.01-0.05 for different materials).
|Barium titanate / poly(vinylidene fluoride-
||Phosphonic acid surface-modified BaTiO3 nanoparticles||35||30-50 nm
|Barium titanate/polyimide (BaTiO3/PI); volume concentration < 40%||Core-shell structure; polyamic acid (PAA) was used to cover particle||20||70-100 nm
|Poly(vinylidene fluoride)/ Barium titanate (PVDF/ BaTiO3); volume concentration
|Surface hydroxylated BaTiO3||18-25||85-100 nm|||
|Barium titanate/polyimide (BaTiO3/PI); volume concentration < 50%||BaTiO3 nanoparticles were prepared by the alkoxide route||30||30-50 nm
|Barium titanate/poly(methyl methacrylate) (BaTiO3/PMMA); volume concentration 53%||BaTiO3 nanoparticles were modified with a silane coupling agent (3-methacryloxypropyltrimethoxysilane)||36||16-21 nm|||
|Barium titanate/polyimide (BaTiO3/PI); volume concentration 59%||BaTiO3 nanoparticles are surface modified by phthalimide with the aid of a silane coupling agent as a scaffold||37||20 nm|||
3.2. Ferroelectric nanoparticles and liquid crystals: Display and non-display applications
It is an established fact that modern technologies require novel and highly advanced materials. During the last decade, nanochemistry has developed a dozen conceptually different pathways of synthesis to satisfy the constantly growing demand for new materials . However, chemical methods are elaborate, time consuming, and expensive. Although they are generally accepted as universal, nanochemistry methods do not work perfectly in certain cases. For example, it’s very difficult (but not impossible) to produce 5-10 nm ferroelectric nanoparticles with tetragonal structures through chemical methods (see Table 2). In many cases, the chemical methods used to produce novel materials can be efficiently supplemented or even replaced with non-synthetic ones. The addition of ferroelectric nanoparticles to different materials (polymers; see Table 6, liquids, liquid crystals etc.) is a good example of a non-synthetic method used to develop materials with improved properties. This subsection will discuss how ferroelectric nanoparticles can modify properties of liquid crystals – materials that found numerous applications in the display industry, photonics, optical processing, and the biotech industry.
The concept of ferroelectric colloids in liquid crystals was created by Yu. Reznikov and coauthors  – liquid crystal material was doped with stabilized ferroelectric nanoparticles of low concentration (~0.3 %). Ferroelectric nanoparticles share their intrinsic properties with the liquid crystals matrix due to the alignment within the liquid crystal and interactions between mesogenic molecules. The low concentration of nanoparticles and their stabilization with surfactant (oleic acid) provided the stability of such systems. This classic paper reported on the main features of such colloids: (1) a lower threshold voltage by a factor of 1.7; (2) an enhanced dielectric anisotropy by a factor of 2; (3) a linear electro-optical response (the sensitivity to the sign of an applied electric field). It should be pointed out that pure nematics are not sensitive to the sign of an electric field – this property is intrinsic to ferroelectric liquid crystals rather than to nematics. The first experimental results stimulated a very active global interest in the field. More than 100 papers were published during the last decade, and, in the last few years, several review papers summarized the most important results [18, 54, 55]. The review paper  published this year by the founder of this field is of special interest since it comprehensively discusses the past, the present, and the future of the liquid crystal colloids.
Ferroelectric nanoparticles embedded into a liquid crystal host strongly interact with the surrounding mesogenic molecules, due to the strong permanent electric field of this particle. These interactions can affect the basic physical parameters of liquid crystals: birefringence, dielectric permittivity, elastic constants, viscosity, electrical and thermal conductivity, temperatures of phase transitions, etc. There are two basic mechanisms responsible for the observed effects: (1) the increase of the orientation coupling between mesogenic molecules; and (2) the direct contribution of the permanent polarization of the particle . Experimental data suggests that the first scenario (the increase of the orientation coupling between mesogenic molecules) is more likely to happen in the case of single component liquid crystals . The second mechanism (associated with the direct contribution of the permanent polarization of the ferroelectric nanoparticle to the physical properties of liquid crystals) is the primary factor in the case of multi-component liquid crystal mixtures .
So far most of the reported experimental data describes the properties of multi-component nematics: liquid crystals doped with ferroelectric nanoparticles. The electric field generated by ferroelectric nanoparticles can cause micro- and/or nano-separation of such mixturesandaffect the macroscopic properties of the liquid crystal colloid. As a result, in some cases, the data found for single component liquid crystals (5CB) is different from the data obtained for multi-component mixtures. Nevertheless, an analysis of the existing literature  shows that most of the published experimental data report that ferroelectric nanoparticles embedded in liquid crystals at low concentrations: (1) enhance dielectric permittivity, dielectric anisotropy, and optical birefringence; (2) lower the switching voltage Uth for the Freedericksz transition; (3) increase the orientational order parameter
The stability of liquid crystal colloids is the most challenging problem that prevents the transition of liquid crystal colloids of ferroelectric nanoparticles from the academic sector to the industrial domain. During the last few years, the general focus of the research has shifted toward this problem, and the proper surface functionalization of nanoparticles is now being considered as one of the most important factors affecting the stability of liquid crystal colloids. The shape and size of nanoparticles are also of the utmost importance – it was found that 10-20 nm ferroelectric nanoparticles affect the properties of a liquid crystal host much morethan the same but larger nanoparticles(~100 nm).
In summary, ferroelectric nanoparticles can modify the intrinsic properties of liquid crystal materials without time-consuming and expensive chemical synthesis. Experimental data on the enhancement of electro-optical, optical, and nonlinear-optical responses of such materials shows the strong potential of ferroelectric nanoparticles for improving the ‘‘practical’’ properties of liquid crystals, especially for those materials where the method of chemical synthesis has reached its limit. Such modified materials are very attractive and suitable for use in switchable lenses, displays, and beam steering, as well as other light-controlling devices (spatial light modulators, tunable filters etc.) .
4. Ferroelectric nanoparticles in biology
In the last decade, ferroelectric nanoparticle areas of application veered toward biology and medicine. The first challenge to address when introducing nanoparticles to biological and medical systems is how to make them stable in media that is bio-compatible, namely in aqueous solutions. If the ferroelectric nanoparticles are not coated with a stabilizing agent, the intrinsic properties of such nanoparticles very often lead to unwanted effects such as aggregation and precipitation, as well as the leaching of some ions (leading to change in particle properties) in aqueous solutions. There has been a tremendous amount of effort in the last twenty years to create many species of ferroelectric nanoparticles with different surface coatings [56and references within]. For example, such stabilizing agents as polyacrylic acid, polymethacrylic acid, polyaspartic acid, (aminomethyl) phosphonic acid and poly-l-lysine were tried on barium titanate nanoparticles. A large variety of possible coatings yields different surface properties of said nanoparticles – different thickness and charge of the surface layer, different strength of stabilizing agent adhesion, different resulting particle size – all of it leading to very different interactions with biological objects such as cells and cellular components. Such water-soluble ferroelectric nanoparticles can be further functionalized with fluorescent markers or antibodies , and they have been recently observed within a number of mammalian cells [58, 59, 60] in vitro. The majority of ferroelectric nanoparticles that have been successfully functionalized are in the middle of nano size range (~100 nm or more), and the surface functionalization very frequently adds a thick surface layer, resulting in particles that are a few hundred nanometers in size. This poses a challenge which a few researchers are attempting to overcome through bio-inspired surfactants . The surface functionalization of nanoparticles can be crucial for a desired effect in a biosystem – the response is often cell-specific, and biocompatibilty has to be experimentally tested for each new combination of nanoparticle and cell . For example, a recent study  indicates that larger (over 200 nm) barium titanate nanoparticles have been successfully used with and without surface modification and they cause no toxic response in endothelial cell cultures.
Current efforts in this area concentrate on carrying these findings through to the systems of cells and tissue in vivo [63, 64]. Such biocompatible nanoparticles can be used in a variety of ways: as imaging agents [58, 59, 60, 64, 65], biocompatible nanoprobes [62, 66, 67, 68], cell proliferation agents , etc. Ferroelectric nanoparticles are currently being widely explored for applications in the area of medical imaging, e.g. for enhancing contrast in second harmonic generating methods for imaging deep tissue in vitro and in vivo [64, 69] for such important applications as screening for genetic diseases or cancer.
5. Ferroelectric nanoparticles applications in medicine and medical engineering
As mentioned above, ferroelectric nanoparticles have become widely used in material science and engineering applications, but biological and medical applications of these fascinating nanoparticles has only begun to be explored in the last decade. It has been recently discovered that they can be used for cell imaging or the detection of malignancies in lung cancer studies, or they can be functionalized to induce cell proliferation. Ferroelectric materials have a non-centrosymmetric crystalline structure, and are thus capable of generating a second harmonic of light . This distinctive feature of ferroelectrics is the basis for a growing number of applications of ferroelectric nanoparticles as imaging/diagnostic agents and nanoprobes in optical imaging .
Optical imaging and detection methods are the most widespread among biological and medical communities. For example, second harmonic generation imaging has been successfully used for detection of
The intrinsic large values of the dielectric permittivities of ferroelectric nanoparticles suggest their use to enhance the dielectric contrast of materials, such as polymers [77 and references within] and biological tissue . These unique properties of ferroelectric nanoparticles lead to their novel use as contrast-enhancing agents for microwave tomography, which is a method of non-invasive assessment and diagnostics of soft tissues (such as detecting malignancies).Recently, ferroelectric electro spun nanofibers also emerged in various biomedical areas including medical prostheses, tissue engineering, wound dressing, and drug delivery [28,29,30].
In conclusion, ferroelectric materials found a wide variety of biomedical applications in the last decade – and the list is constantly growing . The ferroelectric material (e.g. barium titanate) used in medical implants has been known to accelerate osteogenesis , and the same material in nanoparticle form works both as an SHG probe to detect Osteogenesis Imperfecta  and, through microwave tomography, to detect lung cancer . We expect more applications will become possible if other effects, such as piezoelectricity, ferroelectric hysteresis or stress-birefringence coupling, are exploited with biology and medicine in mind.
A review of recently published research papers allows us to conclude that the unique properties of ferroelectric nanoparticles offer an enormous range of applications, especially in material technologies, biology, and medicine. However, since such a conclusion has become an academic cliché, we would like to make just a few realistic and optimistic comments on the subject.
Discussing any application, we have to be more specific and distinguish between potential applications and actual (i.e. mass commercialized) ones. So far, the “applied” field of ferroelectric nanoparticles is at the stage of high potential for commercialization rather than real mass-commercialization. However, after the very first proof-of-concept research studies were completed just recently, a serious shift toward real applications was initiated. The research community realized that the controllable preparation of nanoparticles (size, shape), their proper surface functionalization, and the homogeneous dispersion into host material (liquid crystals, polymers, biological species) are among the most critical steps on the way to mass-commercialization. Many applications (especially bio-medical) require a large-scale preparation of mono-dispersed, very fine (5-10 nm) ferroelectric nanoparticles in the tetragonal phase – and only recently has substantial progress been made in this direction (see section 2). However, such ultra-fine nanoparticles were mostly tested in material technologies (ferroelectric liquid crystal colloids), while bio-medical methods utilized relatively large ferroelectric nanoparticles (~50-100 nm) (sections 4-5). The bioconjugation of 5-10 nm ferroelectric nanoparticles can extend the area of biomedical application even more, since these nanoparticles can be used as both passive and active nanoprobes.
The applied science of ferroelectric nanoparticles is in the beginning of its development. Many fundamental and applied problems still need to be solved before the potential applications will be converted into actual ones. Nevertheless, despite the fact that the emerging problems in applying nanoparticles in material technologies and biomedicine are still numerous , we can conclude that a good balance between purely academic and purely applied foci of research is the key toward mass commercialization of ferroelectric nanoparticles in all applied fields mentioned above.
The authors are very grateful to all coauthors of the papers related to the topic of ferroelectric nanoparticles. We acknowledge also the support of the UCCS Center for the Biofrontiers Institute, University of Colorado at Colorado Springs. A great portion of the work described in this review has been supported by the grants from the NSF #1102332 “Liquid Crystal Signal Processing Devices for Microwave and Millimeter Wave Operation” and # 1010508 “STTR Phase 1: Design, Fabrication, and Characterization of Ferroelectric Nanoparticle Doped Liquid Crystal / Polymer Composites.”
List of abbreviations
AFM atomic force microscopy
DCS differential scanning calorimetry
DLS dynamic light scattering
DTA differential thermal analysis
EDX energy dispersive X-rayspectroscopy
EFM electrostatic force microscopy
FE-SEM field-emission scanning electron microscopy
FTIR Fourier transform infrared spectroscopy
HRTEM high resolution transmission electron microscopy
MLCC multilayer ceramic capacitors
PAA polyamic acid
PTCR positive temperature coefficient of resistance
PMMA poly(methyl methacrylate)
PVDF poly(vinylidene fluoride)
SAED selected area electron diffraction
SEM scanning electron microscopy
SHG probe second harmonic generating probe
SMPS scanning mobility particle size
SPM scanning probe microscopy
TEM transmission electron microscopy
TG or TGA thermo gravimetric analysis
XPSX-ray photoelectron spectroscopy
Haertling, G.H. Ferroelectric ceramics: history and technology. Journal of the American Ceramic Society82, 797-818 (1999).
Cross, L.E. & Newnham, R.E. in High-Technology Ceramics—Past, Present,and Future289–305 (American Ceramic Society, Westerville, OH, 1987).
Mitsui, T. in Springer Handbook of Condensed Matter and Materials Data (ed. Warlimont, W.M.a.H.) 903 – 938 (Springer, Berlin, 2006).
Whatmore, R. in Springer Handbook of Electronic and Photonic Materials (ed. Capper, S.K.a.P.) 597 – 623 (Springer, Berlin, 2006).
Kalinin, S.V. et al. Nanoscale Electromechanics of Ferroelectric and Biological Systems: A New Dimension in Scanning Probe Microscopy. Annual Review of Materials Research37, 189-238 (2007).
Gruverman, A. & Kholkin, A. Nanoscale ferroelectrics: processing, characterization and future trends. Reports on Progress in Physics69, 2443-74 (2006).
Ahn, C.H., Rabe, K.M. & Triscone, J.M. Ferroelectricity at the nanoscale: local polarization in oxide thin films and heterostructures. Science303, 488-91 (2004).
Scott, J.F. Applications of modern ferroelectrics. Science315, 954-9 (2007).
Sarkar, D. Synthesis and Properties of BaTiO3 Nanopowders. Journal of the American Ceramic Society94, 106-110 (2011).
Zhu, Y.-F., Zhang, L., Natsuki, T., Fu, Y.-Q. & Ni, Q.-Q. Facile Synthesis of BaTiO3 Nanotubes and Their Microwave Absorption Properties. ACS Applied Materials & Interfaces4, 2101-2106 (2012).
O'Brien, S., Brus, L. & Murray, C.B. Synthesis of Monodisperse Nanoparticles of Barium Titanate: Toward a Generalized Strategy of Oxide Nanoparticle Synthesis. Journal of the American Chemical Society123, 12085-12086 (2001).
Buscaglia, M.T., Bassoli, M., Buscaglia, V. & Vormberg, R. Solid-State Synthesis of Nanocrystalline BaTiO3: Reaction Kinetics and Powder Properties. Journal of the American Ceramic Society91, 2862-2869 (2008).
Zhang, Y., Wang, L. & Xue, D. Molten salt route of well dispersive barium titanate nanoparticles. Powder Technology217, 629-633 (2012).
Wei, X. et al. Synthesis of Highly Dispersed Barium Titanate Nanoparticles by a Novel Solvothermal Method. Journal of the American Ceramic Society91, 315-318 (2008).
Hayashi, H. & Hakuta, Y. Hydrothermal Synthesis of Metal Oxide Nanoparticles in Supercritical Water. Materials3, 3794-3817 (2010).
Zhang, H. et al. Fabrication of Monodispersed 5-nm BaTiO3 Nanocrystals with Narrow Size Distribution via One-Step Solvothermal Route. Journal of the American Ceramic Society94, 3220-3222 (2011).
Atkuri, H. et al. Preparation of ferroelectric nanoparticles for their use in liquid crystalline colloids. Journal of Optics A: Pure and Applied Optics11, 024006 (2009).
Garbovskiy, Y. & Glushchenko, A. in Solid State Physics (ed. Camley, R.E.) 1 – 74 (2010).
Cook, G. et al. Nanoparticle doped organic-inorganic hybridphotorefractives. Optics Express16, 4015-4022 (2008).
Cook, G. et al. Harvesting single ferroelectric domain stressed nanoparticles for optical and ferroic applications. Journal of Applied Physics108, 064309-4 (2010).
Basun, S.A., Cook, G., Reshetnyak, V.Y., Glushchenko, A.V. & Evans, D.R. Dipole moment and spontaneous polarization of ferroelectric nanoparticles in a nonpolar fluid suspension. Physical Review B84, 024105 (2011).
Swaminathan, V. et al. Microwave synthesis of noncentrosymmetric BaTiO3 truncated nanocubes for charge storage applications. ACS Appl Mater Interfaces2, 3037-42 (2010).
Fuentes, S. et al. Synthesis and characterization of BaTiO3 nanoparticles in oxygenatmosphere. 505, 568–572 (2010).
Qi, J.Q. et al. Direct synthesis of ultrafine tetragonal BaTiO3 nanoparticles at room temperature. Nanoscale Research Letters6, 466 (2011).
Kong, L.B., Zhang, T.S., Ma, J. & Boey, F. Progress in synthesis of ferroelectricceramicmaterialsviahigh-energymechanochemicaltechnique. 53, 207–322 (2008).
Dang, F. et al. Aneweffect of ultrasonication on the formation of BaTiO3 nanoparticles. 17, 310–314 (2010).
Suzuki, K. & Kijima, K. Well-crystallized barium titanate nanoparticles prepared by plasma chemical vapor deposition. 58, 1650–1654 (2004).
Ramaseshan, R., Sundarrajan, S., Jose, R. & Ramakrishna, S. Nanostructured ceramics by electrospinning. Journal of Applied Physics102, 111101-17 (2007).
He, Y. et al. Humidity sensing properties of BaTiO3 nanofiber prepared via electrospinning. Sensors and Actuators B: Chemical146, 98-102 (2010).
Dai, Y., Liu, W., Formo, E., Sun, Y. & Xia, Y. Ceramic nanofibers fabricated by electrospinning and their applications in catalysis, environmental science, and energy technology. Polymers for Advanced Technologies22, 326-338 (2011).
Jung, D.S., Hong, S.K., Cho, J.S. & Kang, Y.C. Nano-sizedbariumtitanatepowders with tetragonalcrystalstructureprepared by flamespraypyrolysis. 28, 109–115 (2008).
Li, X., Xu, H., Chen, Z.-S. & Chen, G. Biosynthesis of Nanoparticles by Microorganisms and Their Applications. Journal of Nanomaterials2011 (2011).
Chen, C.-L. & Rosi, N.L. Peptide-Based Methods for the Preparation of Nanostructured Inorganic Materials. Angewandte Chemie International Edition49, 1924-1942 (2010).
Briggs, B.D. & Knecht, M.R. Nanotechnology Meets Biology: Peptide-based Methods for the Fabrication of Functional Materials. The Journal of Physical Chemistry Letters3, 405-418 (2012).
Dhillon, G.S., Brar, S.K., Kaur, S. & Verma, M. Green approach for nanoparticle biosynthesis by fungi: current trends and applications. Critical Reviews in Biotechnology32, 49-73 (2011).
Beier, C.W., Cuevas, M.A. & Brutchey, R.L. Room-Temperature Synthetic Pathways to Barium Titanate Nanocrystals. Small4, 2102-2106 (2008).
Ahmad, G. et al. Rapid Bioenabled Formation of Ferroelectric BaTiO3 at Room Temperature from an Aqueous Salt Solution at Near Neutral pH. Journal of the American Chemical Society130, 4-5 (2007).
Jha, A.K. & Prasad, K. Ferroelectric BaTiO3 nanoparticles: Biosynthesis and characterization. Colloids and Surfaces B: Biointerfaces75, 330-334 (2010).
Bansal, V., Poddar, P., Ahmad, A. & Sastry, M. Room-Temperature Biosynthesis of Ferroelectric Barium Titanate Nanoparticles. Journal of the American Chemical Society128, 11958-11963 (2006).
Nuraje, N. et al. Room Temperature Synthesis of Ferroelectric Barium Titanate Nanoparticles Using Peptide Nanorings as Templates. Advanced Materials18, 807-811 (2006).
Jha, A.K. & Prasad, K. Synthesis of BaTiO3 nanoparticles: A new sustainable green approach. Integrated Ferroelectrics117, 49-54 (2010).
Ould-Ely, T. et al. Large-scale engineered synthesis of BaTiO3 nanoparticles using low-temperature bioinspired principles. Nature Protocols6, 97-104 (2011).
Bansal, V., Bharde, A., Ramanathan, R. & Bhargava, S.K. Inorganic materials using ‘unusual’ microorganisms. Advances in Colloid and Interface Science.
Kamiya, H. et al. Preparation of Highly Dispersed Ultrafine Barium Titanate Powder by Using Microbial‐Derived Surfactant. Journal of the American Ceramic Society86, 2011-2018 (2012).
Pithan, C., Hennings, D. & Waser, R. Progress in the Synthesis of Nanocrystalline BaTiO3 Powders for MLCC. International Journal of Applied Ceramic Technology2, 1-14 (2005).
Kim, P. et al. High Energy Density Nanocomposites Based on Surface-Modified BaTiO3 and a Ferroelectric Polymer. ACS Nano3, 2581-2592 (2009).
Dang, Z.-M. et al. Fabrication and Dielectric Characterization of Advanced BaTiO3/Polyimide Nanocomposite Films with High Thermal Stability. Advanced Functional Materials18, 1509-1517 (2008).
Zhou, T. et al. Improving Dielectric Properties of BaTiO3/Ferroelectric Polymer Composites by Employing Surface Hydroxylated BaTiO3 Nanoparticles. ACS Applied Materials & Interfaces3, 2184-2188 (2011).
Fan, B.-H., Zha, J.-W., Wang, D.-R., Zhao, J. & Dang, Z.-M. Experimental study and theoretical prediction of dielectric permittivity in BaTiO3/polyimide nanocomposite films. Applied Physics Letters100, 092903-4 (2012).
Nagao, D., Kinoshita, T., Watanabe, A. & Konno, M. Fabrication of highly refractive, transparent BaTiO3/poly(methyl methacrylate) composite films with high permittivities. Polymer International60, 1180-1184 (2011).
Abe, K., Nagao, D., Watanabe, A. & Konno, M. Fabrication of highly refractive barium-titanate-incorporated polyimide nanocomposite films with high permittivity and thermal stability. Polymer International, n/a-n/a (2012).
Balzani, V. Nanochemistry: A Chemical Approach to Nanomaterials. Geoffrey A. Ozin and André C. Arsenault. Small2, 678-679 (2006).
Reznikov, Y. et al. Ferroelectric nematic suspension. Applied Physics Letters82, 1917-1919 (2003).
Reznikov, Y. in Liquid Crystals Beyond Displays: Chemistry, Physics, and Applications (ed. Li, Q.) 403-426 (John Wiley & Sons, Inc., 2012).
Liang, H.-H. & Lee, J.-Y. Enhanced Electro-Optical Properties of Liquid Crystals Devices by Doping with Ferroelectric Nanoparticles. Ferroelectrics - Material Aspects, 193-210 (2011).
Ciofani, G. et al. Preparation of stable dispersion of barium titanate nanoparticles: Potential applications in biomedicine. Colloids and Surfaces B: Biointerfaces76, 535–543 (2010).
Hsieh, C.-L., Grange, R., Pu, Y. & Psaltis, D. Bioconjugation of barium titanate nanocrystals with immunoglobulin G antibody for second harmonic radiation imaging probes. Biomaterials31, 2272–2277 (2010).
Hsieh, C.-L., Grange, R., Pu, Y. & Psaltis, D. (eds. Campagnola, P.J., Stelzer, E.H.K. & von Bally, G.) 73670D-6 (SPIE, Munich, Germany, 2009).
Hsieh, C.-L., Grange, R., Pu, Y. & Psaltis, D. Three-dimensional harmonic holographic microcopy using nanoparticles as probes for cell imaging. Optics Express17, 2880-2891 (2009).
Grange, R., Hsieh, C.L., Pu, Y. & Psaltis, D. in European Conference on Lasers and Electro-Optics 2009 and the European Quantum Electronics Conference. CLEO Europe - EQEC 2009. 1-1 (2009).
Ciofani, G. et al. in Piezoelectric Nanomaterials for Biomedical Applications 213-238 (Springer Berlin Heidelberg, 2012).
Yust, B.G., Razavi, N., Pedraza, F. & Sardar, D.K. (eds. Cartwright, A.N. & Nicolau, D.V.) 82310H-6 (SPIE, San Francisco, California, USA, 2012).
Zipfel, W.R. et al. Live tissue intrinsic emission microscopy using multiphoton-excited native fluorescence and second harmonic generation. Proceedings of the National Academy of Sciences100, 7075-7080 (2003).
Pantazis, P., Maloney, J., Wu, D. & Fraser, S.E. Second harmonic generating (SHG) nanoprobes for in vivo imaging. Proceedings of the National Academy of Sciences107, 14535-14540 (2010).
Ciofani, G., Ricotti, L. & Mattoli, V. Preparation, characterization and in vitro testing of poly(lactic-co-glycolic) acid/barium titanate nanoparticle composites for enhanced cellular proliferation. Biomedical Microdevices13, 255-266 (2011).
Pantazis, P., Pu, Y., Psaltis, D. & Fraser, S. (eds. Periasamy, A. & So, P.T.C.) 71831P-5 (SPIE, San Jose, CA, USA, 2009).
Horiuchi, N. Imaging: Second-harmonic nanoprobes. Nature Photonics5, 7-7 (2011).
Hsieh, C.-L., Grange, R., Pu, Y. & Psaltis, D. (eds. Mohseni, H. & Razeghi, M.) 77590T-6 (SPIE, San Diego, California, USA, 2010).
Hsieh, C.-L., Lanvin, T., Grange, R., Pu, Y. & Psaltis, D. in Conference on Lasers and Electro-Optics (CLEO), 2011 1-2 (2011).
Semenov, S., Pham, N. & Egot-Lemaire, S. in World Congress on Medical Physics and Biomedical Engineering (eds. Dössel, O. & Schlegel, W.C.) 311-313 (Springer Berlin Heidelberg, Munich, Germany, 2009).
Adur, J. et al. (eds. Periasamy, A., Konig, K. & So, P.T.C.) 82263P-7 (SPIE, San Francisco, California, USA, 2012).
Wang, C.-C. et al. Differentiation of normal and cancerous lung tissues by multiphoton imaging. Journal of Biomedical Optics14, 044034-4 (2009).
Chan, W.C.W. in Advances in Experimental Medicine and Biology 208 (Springer Science+Business Media, LLC, 2007).
Dempsey, W.P., Fraser, S.E. & Pantazis, P. SHG nanoprobes: Advancing harmonic imaging in biology. BioEssays34, 351-360 (2012).
Yust, B.G., Sardar, D.K. & Tsin, A. (eds. Cartwright, A.N. & Nicolau, D.V.) 79080G-7 (SPIE, San Francisco, California, USA, 2011).
Ganeev, R.A., Suzuki, M., Baba, M., Ichihara, M. & Kuroda, H. Low- and high-order nonlinear optical properties of BaTiO3 and SrTiO3 nanoparticles. Journal of the Optical Society of America B25, 325-333 (2008).
Lai, K.T., Nair, B.G. & Semenov, S. Optical and microwave studies of ferroelectric nanoparticles for application in biomedical imaging. Microwave and Optical Technology Letters54, 11-13 (2012).
Ciofani, G. et al. 987-990 (KINTEX, Korea, 2010).
Furuya, K., Morita, Y., Tanaka, K., Katayama, T. & Nakamachi, E. (eds. Martin-Palma, R.J. & Lakhtakia, A.) 79750U-6 (SPIE, San Diego, California, USA, 2011).
Florence, A.T. “Targeting” nanoparticles: The constraints of physical laws and physical barriers. (2012).